technical report documentation page

TECHNICAL REPORT DOCUMENTATION PAGE1. Report No.2. Government Accession No. 3. Recipient's Catalog No.RDT RI00-002B4. Title and Subtitle5. Report DateCreep, Shrinkage and CTE Evaluation: MoDOT’s New Bridge Deck MixCompanion Testing to HPC Bridge DeckFebruary 20056. Performing Organization CodeUniversity of Missouri-Rolla7. Author(s)Nidhi, Joshi, John Myers, Juan La Gamma – University of Missouri-Rolla8. Performing Organization Report No.RDT RI00-002B9. Performing Organization Name and AddressUniversity of Missouri-RollaDept. of Civil, Architectural and Environmental Engineering211 Butler-Carlton HallRolla, Missouri 65409-003012. Sponsoring Agency Name and AddressMissouri Department of TransportationResearch, Development and Technology Division10. Work Unit No.11. Contract or Grant No.13. Type of Report and Period CoveredFinal Report, February 200514. Sponsoring Agency CodeMoDOTP. O. Box 270-Jefferson City, MO 6510215. Supplementary NotesThe investigation was conducted in cooperation with the University Transportation Center at University of Missouri – Rolla.16. AbstractMoDOT RDT Research Project R-I00-002 “HPC for Bridge A6130 – Route 412 Pemiscot County” was recentlycompleted in June of 2004 [Myers and Yang, 2004]. Among other research tasks, part of this research study investigated thecreep, shrinkage and coefficient of thermal expansion (CTE) of Missouri’s first high performance concrete (HPC) superstructurebridge. This study examined these aforementioned properties on both the prestressed concrete (PC) girders and the cast-in-place(CIP) deck which both utilized HPC on this aforementioned project.In 2003 the Missouri Department of Transportation (MoDOT) studied nine different mix designs for possible use inbridge deck applications [MoDOT Report RI01-044, 2003]. The objective of this internal MoDOT study was to reduce thecontent of cementitious material to reduce shrinkage, but maintain good durability characteristics. Of the original nine mixdesigns, one was ultimately selected for use in an actual bridge deck application, namely, MoDOT Bridge A6671 nearWaynesville, Missouri. There was interest to study how the mix design used in this bridge compared to the previous HPC deckmix design used in Bridge A6130.The objectives of this research, project study R-I00-002B, were to:1. Determine the creep, shrinkage and CTE properties of the MoDOT Bridge A6671 deck mix.2. Data analysis and curve fitting of the data obtained from MoDOT Bridge A6671 deck mix.3. Compare the properties with those of the HPC Bridge A6130 (near Hayti, Missouri) deck mix to gain anunderstanding of the variation that may be expected in these two deck mixes.The primary difference between the two mix designs was the cementitious content. The coarse aggregate content alsovaried to some degree. The variation between the creep, shrinkage and coefficient of thermal expansion properties of the twomix designs are presented and discussed. The findings and conclusions of the study are also presented.17. Key WordsCreepShrinkageCTEBridge DeckMix ProportioningHigh Performance Concrete19. Security Classification (of this **report**)Unclassified20. Security Classification (of this **page**)Unclassified18. Distribution StatementNo restrictions. This document is available to the publicthrough National Technical Information Center, Springfield,Virginia 2216121. No. of Pages3922. PriceForm DOT F 1700.7 (06/98)

Investigation Number RI00-002BFinal Report forCreep, Shrinkage and CTE Evaluation: MoDOT’s New Bridge Deck MixCompanion Testing to HPC Bridge DeckDEPT. OF CIVIL, ARCH. & ENVIR. ENGINEERINGUNIVERSITY OF MISSOURI-ROLLAFebruary 2005i

LIST OF CONTENTS LIST OF FIGURES iiiLIST OF TABLES iii1. INTRODUCTION 11.1 GENERAL DESCRIPTION 11.2 BACKGROUND AND OBJECTIVE 12. LITERATURE AND BACKGROUND2.1 CREEP 3 2.2 SHRINKAGE 9 2.3 COEFFICIENT OF THERMAL EXPANSION 14 3. FABRICATION AND DESIGN3.1 SPECIMEN FABRICATION AND MIX DESIGN 16 3.2 MIX CONSTITUENTS AND PROPORTIONS 22 4. EXPERIMENTAL RESULTS4.1 RESULTS FOR CREEP TEST 25 4.2 RESULTS FOR SHRINKAGE TEST 27 4.3 RESULTS FOR CTE TEST 29 5. COMPARISION OF BRIDGE A6671 TO BRIDGE A61305.1 COMPARISON OF CREEP RESULTS 30 5.2 COMPARISION OF SHRINKAGE RESULTS 31 5.3 COMPARISION OF CTE RESULTS 33 6. CONCLUSIONS AND RECOMMENDATIONS 35 REFERENCES 37 ii

LIST OF FIGURES3.1 C/S/T Specimens and DEMEC Points Arrangements 183.2 Creep Loading Frame and Specimen 193.3 Creep Loading Frames and Specimens 204.1 Individual Behavior of three Creep Specimens 254.2 Individual Behavior of three Creep Specimens 264.3 Individual Behavior of four Shrinkage Specimens 274.4 Individual Behavior of four Shrinkage Specimens 285.1 Creep Comparison Curve 315.2 Shrinkage Comparison Curve 335.3 CTE Comparison Curve 34LIST OF TABLES3.1 Specimen for C/S/T 163.2 Comparison of the two Deck Mixes 244.1 Creep-Time Regression Curve Parameters (General Form) 274.2 Shrinkage-Time Regression Curve Parameters (General Form) 285.1 Comparison of Creep Curve Parameters 305.2 Comparison of Shrinkage Curve Parameters 325.3 Average value of CTE for both the Deck Mixes 33iii

1.1 General Description1. INTRODUCTIONCreep, shrinkage and coefficient of thermal expansion (CTE) are important for bothconventional and high performance concrete (HPC). Creep is defined as continueddeformation under a constant stress. Mix composition, curing condition, loadingconditions, member geometry, service exposure conditions and amount of reinforcing aremajor factors affecting creep.Shrinkage is broadly defined as the decrease in volume of a concrete element as itloses moisture by evaporation. The major factors affecting drying shrinkage are curingconditions, member size, member shape, amount of reinforcing, temperature, and mixcomposition like aggregate, w/cm ratio, admixtures.The coefficient of thermal expansion (CTE) of concrete is a function of thecoefficients of both the aggregate and paste. Since aggregates generally make up bulk ofthe concrete mix, the coefficient of thermal expansion of concrete is most influenced bythe coefficient of the aggregate, as well as the quantity of aggregate in the mix.Each of these characteristics is an important consideration when predicting bothultimate strength capacity and serviceability of prestressed concrete elements.1.2 Project Background and ObjectiveMoDOT RDT Research Project R-I00-002 “HPC for Bridge A6130 – Route 412Pemiscot County” was recently completed in June of 2004 [Myers and Yang, 2004].Among other research tasks, part of this research study investigated the creep, shrinkageand coefficient of thermal expansion (CTE) of Missouri’s first high performance concrete(HPC) superstructure bridge. This study examined these aforementioned properties onboth the prestressed concrete (PC) girders and the cast-in-place (CIP) deck which bothutilized HPC on this aforementioned project.In 2003 the Missouri Department of Transportation (MoDOT) studied nine differentmix designs for possible use in bridge deck applications [MoDOT Report RI01-044,2003]. The objective of this internal MoDOT study was to reduce the content of1

cementitious material to reduce shrinkage, but maintain good durability characteristics.Of the original nine mix designs, one was ultimately selected for use in an actual bridgedeck application, namely, MoDOT Bridge A6671 near Waynesville, Missouri. There wasinterest to study how the mix design used in this bridge compared to the previous HPCdeck mix design used in Bridge A6130.The objectives of this research, project study R-I00-002B, were to:1. Determine the creep, shrinkage and CTE properties of the MoDOT Bridge A6671deck mix.2. Data analysis and curve fitting of the data obtained from MoDOT Bridge A6671deck mix.3. Compare the properties with those of the HPC Bridge A6130 (near Hayti,Missouri) deck mix to gain an understanding of the variation that may beexpected in these two deck mixes.The primary difference between the two mix designs was the cementitious content. Thecoarse aggregate content also varied to some degree.2

2.1 Creep2. LITERATURE AND BACKGROUNDCreep of concrete can broadly be defined as the time-dependent increase in strainunder a sustained stress. Total creep actually consists of two components: basic creep anddrying creep. Basic creep is the creep occurring with no moisture exchange between theconcrete and its surroundings, while drying creep can be defined as the creep dependenton loss of moisture to the environment [Libby, J.R., 1990]. Basic creep is generallyassociated with the movement and rearrangement of adsorbed water layers, and dryingcreep is associated with the loss of evaporable water [Ngab, A.S., 1981].For most engineering applications, it is not necessary to distinguish between basicand drying creep. However, it is important to note that creep and shrinkage are notindependent since drying creep is moisture-dependent, and thus influenced by shrinkage[Neville, A.M., 1983]. As a result, creep and shrinkage strains cannot truly besuperimposed (i.e. the total time-dependent strain is not equal to the algebraic sum of thebasic creep, drying creep, and shrinkage strains). For practical purposes, however, creepcan be defined as the time-dependent change in strain of concrete under sustained load,less the shrinkage (and thermal) strain occurring on unstressed concrete in the sameenvironmental conditions. This approach has been used by ACI Committee 209 [1992]and in numerous past experimental studies, and allows for the superposition of creep andshrinkage strains in time-dependent analyses.It is often useful to quantify creep of concrete in forms other than the total creepstrain, ε c . The two most common forms are specific creep, η c , and creep coefficient, C c .Specific creep is sometimes called the “unit creep strain”, and is defined as the creepstrain per unit stress:ε cη = ................................Equation 2.1cσ3

The creep coefficient is defined as the ratio of the time-dependent creep strain to theinitial elastic strain, ε i :ε cC = ................................Equation 2.2cε iThus, a creep coefficient of 2.0 implies that the total strain due to initial elastic loadresponse and time-dependent creep is three times the initial elastic strain. The specificcreep and creep coefficient can be related by the following equation, where E c is taken asthe modulus of elasticity at the time of loading:C = E ⋅η ..........................Equation 2.3 c c cMany factors have been shown to influence creep of concrete. These factors cangenerally be categorized as mix composition factors and other factors related to curing,service exposure conditions, loading conditions, and member geometry. Because so manyfactors influence creep, the magnitude of creep strains will vary greatly between differentconcretes under different conditions.Creep essentially occurs in the paste of concrete, and the aggregate acts to restrainthe creep of the paste. As a result, the quantity and stiffness (modulus of elasticity) of thecoarse aggregate will influence the creep behavior of the concrete to some extent [Neville,A.M., 1981]. Many attempts have been made in the literature to relate creep to water-tocement(water-to-binder) ratio, cement content, cement type, water content, fineaggregate content, and other paste properties, but the interdependence of such propertieshas resulted in conflicting data concerning their effects [Mindess, S. and Young, J.F.,1981]. Some authors argue that creep is essentially related to the stress-strength ratio(ratio of the applied stress to the concrete strength at time of loading), whichencompasses the net effects of the previously mentioned interdependent paste properties[Neville, 1981 and 1983].However, it is generally agreed upon that concretes with lower water-to-cement(water-to-binder) ratios exhibit less creep than similar concretes with higher water-tocement(water-to-binder) ratios. Studies of experimental data have shown this trend to beespecially true when corrections are made to account for differences in quantities ofcement paste. That is, concretes with lower water-to-cement (water-to-binder) ratios and4

the same paste content exhibit lower creep. This conclusion could also be interpreted asdemonstrating the influence of water content. Concretes with less water tend to exhibitlower creep.Loading factors that influence creep behavior include the age of the concrete atloading and magnitude of the applied load. Both of these factors contribute to the stressstrengthratio mentioned in preceding paragraphs. It has been well established thatconcrete creeps more when loaded at earlier ages. Likewise, higher loads result in morecreep strain for a given concrete. A linear relationship between creep strain andmagnitude of applied stress is known to exist up to a given level of stress. The upperstress limit of the linear relationship is generally **report**ed as about 50% to 60% of thecompressive strength for most concretes. Above this stress, microcracking may occur andthe relationship may become nonlinear [Gilbert, R.I., 1988]. At stress levels approachingthe ultimate strength of the concrete, creep can eventually lead to failure. The stress levelabove which this occurs is commonly referred to as the sustained load strength.Other factors that can influence creep of concrete include curing and serviceexposure conditions. Duration and type of curing can affect creep by influencing theconcrete strength (and thus the stress-strength ratio) at the time of loading. Relativehumidity can greatly affect creep, or more precisely, the magnitude of drying creep.Lower relative humidity typically results in significantly increased creep [Neville andBrooks, 1990]. Temperature also influences creep, although for most typical applicationsit is considered to be a less important environmental factor than relative humidity. Overthe range of temperatures applicable to most concrete structures (0 to 70°C [32 to 160°F]),creep increases with increasing temperature [Neville, 1981].Tests have also shown that the size and shape of a concrete member or specimencan greatly influence its creep, both in terms of the rate of creep and magnitude ofultimate creep [Hansen and Mattock, 1969]. For larger members, the rate of creep andmagnitude of ultimate creep are significantly smaller, and the magnitude of total creepapproaches the magnitude of basic creep since very little moisture can be lost to theenvironment. This member size and shape influence has generally been expressed byrelating creep to either volume-to-surface ratio, or to a minimum or average memberthickness [1992].5

There is general agreement that creep is less for high strength concretes than forconventional or normal strength concretes. This trend would be expected given thegenerally low water-to-cement (water-to-binder) ratios of most high strength concretes.ACI Committee 363 [1992] identifies several studies where less creep was measured forHSC than for comparable normal-strength concretes. Parrot [1969] observed a 25 percentlower creep coefficient in high strength concrete under drying conditions, whencompared to normal strength concrete loaded to a similar load ratio (30 percent of theconcrete strength). Ngab et al. [1981] found that the specific creep and creep coefficientof high strength concrete with a water-to-cement ratio of 0.32 were respectively 20 to 25percent and 50 to 75 percent that of normal strength concrete made with similar materialsand a water-to-cement ratio of 0.64. Smadi et al. [1987] also observed substantially lesscreep for high strength concretes with compressive strengths of 59 to 69 MPa (8,500 to10,000 psi) and a water-to-cement ratio of 0.32, when compared to low and mediumstrength concretes (compressive strengths less than 41 MPa [6,000 psi]) with water-tocementratios of 0.87 and 0.64, respectively.The Smadi et al. [1987] study also noted that a higher limit exists for high strengthconcrete for the linear relationship between level of stress and creep strain. This limit wasobserved to be approximately 65 percent of the compressive strength for HSC, ascompared to 45 percent for low and medium strength concretes. Similarly, it wasobserved that HSC has a higher sustained loading strength. The stress at which creepstrains lead to failure was found to be 80 percent of the strength for HSC and 75 percentof the strength for low and medium strength concretes.The effect on creep of mineral and chemical admixtures, which are commonly usedin HPC, is somewhat unclear. Brooks and Neville [1992] suggest that few generalizationscan be made concerning their effects on creep, in part because available experimentaldata covers a wide range of test conditions. It is also important to recognize the indirecteffect that admixtures have on creep with respect to the manner in which they influenceother creep-influencing parameters (i.e. water-to-cement/water-to-binder ratio,slump/water content, strength, etc.). Nasser and Al-Manaseer [1986] found that creep of28 MPa (4000 psi) concrete with superplasticizer and 20% Class C fly ash replacementexhibited 72% more creep than the same concrete without admixtures. Sennour and6

Carrasquillo [1989] observed a slight increase in creep for concretes with varyingpercentages of Class C fly ash replacement, and a slight decrease in creep for concreteswith Class F fly ash. The difference was attributed to the effect of the varying CaOcontents between the two classes of fly ash.Several models have been proposed for predicting creep as a function of time for agiven concrete under a given set of load and exposure conditions. The most commonmethod in use in the United States is probably the ACI 209 [1992] method, which isbased on the work of Branson et al. [1971]. This method allows for the determination ofan ultimate creep coefficient, C cu , either by experimental tests or by assuming andmodifying a base value of 2.35. This base value was determined by analyzing the resultsof 120 specimens from several experimental studies conducted prior to 1970 on normalweight,lightweight, and sand-lightweight concretes [Branson, D.E., 1971]. The assumedbase value is meant to represent a general average for many concretes, and should bemodified using a set of multipliers developed for various factors related to concretecomposition. These factors include slump, fine aggregate percentage, cement content, andair content. The multipliers corresponding to these factors may be found in the ACI 209Committee Report [1992].The corrected (assumed) or experimentally determined ultimate creep coefficient isthen modified using multipliers corresponding to loading, curing, and environmentalconditions. The multiplier for ambient relative humidity is given as:γ = 1.27 − (0.0067 ⋅H) for H ≥ 40 ..............Equation 2.4rhwhere H is the relative humidity in percent. The multiplier γ rh defaults to 1.0 for a“standard” relative humidity of 40 percent. For relative humidity less than 40 percent, noequation is given, but γ rh must be taken as greater than 1.0.A multiplier for size and shape effects may be applied in one of two forms, onerelated to average member thickness and another related to volume-to-surface ratio. Themultiplier corresponding to average member thickness is given as:7

γ = 1.10 − (0.017 ⋅ h) .....................Equation 2.5atfor ultimate creep values, where h is specified as the average member thickness (ininches) of the part of the member under consideration. The constants 1.10 and 0.017 arereplaced by 1.14 and 0.023, respectively, to correct creep values during the first year afterloading. This modification is intended to reflect the greater influence of average memberthickness during the first year after loading.The multiplier for size and shape effects based on volume-to-surface ratio, v/s (ininches), is given by:γ =vs1.5 (in.).2−3 ⋅ ⎡1 + 1.13 e ( .54⎣⋅⋅ v s ) ⎤ ...................Equation 2.6⎦Note that this multiplier becomes 1.0 for the “standard” volume-to-surface ratio ofA correction factor is also suggested to account for loading ages other than 7 daysfor moist-cured concrete and 1 to 3 days for steam-cured concrete. The Equation for thismultiplier may be found in the ACI 209 Committee Report [1992].Once all appropriate correction factors have been applied, the creep coefficient atany time t, C ct , can be determined as a function of the corrected ultimate creepcoefficient, C cu . The following hyperbolic-power expression is used for the relationship,where t is the time in days after casting and t 0 is the time of loading:(t − t ) 0.60C ct=10 + (t − t 0) 0.6⋅ C .................Equation 2.7cuThe form of Equation 2.7 is based on the work of Branson et al. [1971]. Thecoefficients 10 and 0.6 were determined as average values from a set of 120 creep tests.A suggested range of other possible values for these two coefficients, as well as for theultimate creep coefficient, is provided in the ACI 209 Committee Report [1992]. Thegeneral form of Equation 2.7 is given in Equation 2.8:8

c0cC ct= (t − t ) ⋅Ccu..................Equation 2.8d + (t −t 0)Other well-known design-oriented prediction models for creep of concrete includethe 1990 CEB model [1991] and the simplified BP (Bazant-Panula) model [1980]. The1990 CEB model is very similar to the ACI 209 model, and allows for the prediction ofcreep as a function of loading age, loading duration, cement type, relative humidity, andmember size and thickness. One of the primary differences between this model and theACI 209 model is that concrete strength is also considered as a variable in the predictionof creep. A second major difference is that the effects of relative humidity and membersize and thickness on the rate of creep are considered, in addition to the effect of thesevariables on the total or ultimate creep. The lack of consideration of the effects of thesevariables on the rate of creep is one of the major deficiencies of the ACI 209 model.The simplified Bazant-Panula [1980] model is a simplified form of a complexmodel for the prediction of creep. This model was developed using a large database ofmeasured creep values from experimental tests. The interrelation of creep and shrinkageis considered in the BP model, and total creep is separated into terms representing basiccreep and drying creep. One of the interesting features of this model is that concretestrength is the major variable in the model, and appears in the calculation of severalparameters used in the model.2.2 ShrinkageShrinkage can be broadly defined as the decrease in volume (not related to thermaleffects) of hardened concrete with time. In this sense, shrinkage in hardened concrete isto be distinguished from plastic shrinkage, which occurs in concrete prior to setting.Three basic types of shrinkage are generally considered to contribute to the total timedependentdecrease in volume. Drying shrinkage is a result of the loss of moisture overtime, carbonation shrinkage is due to the chemical reaction of hardened cement pastewith atmospheric carbon dioxide, and autogenous shrinkage is due to a self-desiccatingeffect that occurs during hydration [Mast, R.F., 1989].9

Drying shrinkage is generally considered to be the major component of the totalshrinkage in concrete structures [Libby, J.R., 1990]. Still, carbonation shrinkage cangreatly increase the total shrinkage under certain environmental conditions, namely thepresence of high concentrations of CO 2 at intermediate relative humidities. It is alsosuggested that many of the experimental data on drying shrinkage include the effects ofcarbonation shrinkage. Autogenous shrinkage, on the other hand, is typically very small[Neville, 1990]. Fortunately, it is unnecessary to distinguish between these three types ofshrinkage in structural design. Thus, the generic term shrinkage will be used throughoutthe rest of this **report**.As with creep, a number of factors are known to affect shrinkage of concrete. Thesefactors can generally be classified as factors related to mix composition, those related tocuring and service exposure conditions and those related to size and shape of the member.Shrinkage is a property of the paste in concrete. Since the aggregate acts to restrainthe shrinkage of the paste, it plays a major role in determining the magnitude of concreteshrinkage [Mindess, 1981 and Neville 1985]. The proportion of aggregate in the mix, aswell as the stiffness (modulus of elasticity) of the aggregate, are considered by many tobe the most important mix composition factors influencing concrete shrinkage. Water-tocement(water-to-binder) ratio is also generally believed to be proportional to shrinkage,with lower ratios resulting in concrete with lower shrinkage. Water content itself isaccepted to be proportional to shrinkage, but there is disagreement as to whether itsinfluence is direct or indirect. Neville suggests that water content only affects shrinkagein that it influences the proportion of aggregate in the mix. Nilson and Winter [1991]suggest that the influence is more direct, and that the quantity of mix water is the chiefmix-related factor influencing shrinkage. Their observations are based largely on thelinear relationship between mix water and shrinkage strain shown by Troxell et al.[1968].Curing and environmental exposure factors can greatly influence concrete shrinkage.Elevated curing temperatures have been shown to reduce long-term shrinkage in severalstudies [Hanson, 1964, Klieger, 1987 and Sennour, 1989]. Some studies [Swamy 1987]have also indicated that the duration of moist curing can influence long-term shrinkage,and ACI Committee 209 [1992] suggests a modification factor that implies less shrinkagefor longer moist curing periods. Ambient relative humidity under service conditions is10

known to greatly affect concrete shrinkage, primarily because it influences the rate ofmoisture exchange between the concrete and the surrounding atmosphere. Low relativehumidities lead to increased shrinkage. It would similarly be expected that elevatedtemperatures would accelerate drying and thus increase the rate of shrinkage [Gilbert,1988], but this effect is considered to be much less significant than the effect of relativehumidity [ACI 209, 1992].One of the most significant factors influencing concrete shrinkage is the size andshape of the member. Both the rate of shrinkage and the ultimate shrinkage tend todecrease as the member becomes larger [Hansen, 1966]. In smaller (thinner) members,the shrinkage tends to occur rapidly and relatively uniformly. In larger (thicker) members,the rate of shrinkage will be fast near the surface, while shrinkage at the innermost partsof the member may develop very slowly or even be nonexistent. Stresses may develop inlarge members as a result of this differential shrinkage [Mindess, 1981]. The relationshipbetween member geometry and shrinkage is generally modeled using the volume-tosurfaceratio, or the average or minimum member thickness.Experimental data has generally shown no clear trend with respect to shrinkage ofhigh strength concrete, though it is often suggested that the shrinkage of high strengthconcrete is similar to the shrinkage of normal strength concretes [ACI 363, 1992]. Ngabet. al. [1981] noted slightly higher shrinkage for high strength concrete when compared tonormal strength concrete made with similar materials. Smadi et al. [1987] also observedhigher shrinkage for high strength concrete (59 to 69 MPa [8,500 to 10,000 psi]) asopposed to normal strength concrete (35 to 41 MPa [5,000 to 6,000 psi]), but observedless shrinkage for HSC than for concretes with very low strengths concrete (21 to 24 MPa[3,000 to 3,500 psi]). Swamy and Anand [1973] observed a high initial rate of shrinkagefor high strength concrete made with finely ground Portland cement, but noted thatshrinkage strains after two years were approximately equal to values suggested in theCEB code [1970].There are also few conclusions regarding the shrinkage of high performanceconcrete (with or without high strengths), or regarding the effect of mineral and chemicaladmixtures on concrete shrinkage. Brooks and Neville [1992] acknowledge that theeffects of individual admixtures are difficult to identify, and that the small body of11

experimental data indicates varying results. Sennour and Carrasquillo [1989] noted thatthe partial replacement of cement with both Class C and Class F fly ashes resulted in aslight increase in shrinkage, and that greater percentages of replacement led to greaterincreases in shrinkage. El Hindy et. al. [1994] observed less shrinkage in HPC with awater-to-binder ratio of 0.22 and made using a blended cement (7 to 8 percent silica fumeby weight) than in HPC with a water-to-binder ratio of 0.28 and no silica fume.Several models have been proposed for the prediction of concrete shrinkage withtime, most of which incorporate the effects of curing and environmental conditions andmember geometry (size and shape). Some models also consider the effect of mixcomposition on shrinkage. The most widely used model in the United States is probablythe ACI 209 [1992] method, which was developed by Branson et. al. [1971]. This methodrecommends an ultimate shrinkage strain of 780 µε based on an analysis of results from356 experimental tests conducted on normal, lightweight, and sand-lightweight concretes[Brooks, J.J., 1992]. This base value can be modified by a set of multiplierscorresponding to mix composition, or an ultimate shrinkage strain can be determinedfrom experimental tests. Mix composition multipliers may be found in the ACI 209Committee Report [1992], and include considerations for slump, fine aggregatepercentage, cement content, and air content.The ultimate shrinkage strain is then modified using multipliers that account forrelative humidity, member size and shape, and duration of moist curing. Thesemultipliers are similar to those given for creep in Section 2.1, and the notation isconsistent. The multiplier for average ambient relative humidity is given in Equation 2.9and Equation 2.10.12

γ =1.40 − (0.010 ⋅ H) for 40 ≤ H ≤ 80.................Equation 2.9rhγrh=3.00 − (0.030 ⋅H) for H > 80.................Equation 2.10Note that the multiplier becomes 1.0 for the “standard” relative humidity of 40percent, and zero for a relative humidity of 100 percent (implying no shrinkage). NoEquation is given for relative humidities less than 40 percent, but the multiplier must betaken as greater than 1.0 in this case.As for creep, the effect of size and shape effects may be considered by using amultiplier for either average member thickness or for volume-to-surface ratio. Themultiplier for average member thickness is:γat=1.17 − (0.029 ⋅ h).......................Equation 2.11for ultimate shrinkage values. The constants 1.17 and 0.029 are replaced by 1.23and 0.038, respectively, to correct shrinkage values during the first year of drying. Thismodification reflects the greater influence of member thickness during the first year ofdrying.The multiplier for size and shape effects based on volume-to-surface ratio v/s (ininches) is given by:v−γ =1.2 e ( .12 ⋅ s⋅) ........................Equation 2.12vsNote that this multiplier is equal to 1.0 for the “standard” volume-to-surface ratio of1.5 inches.A loading factor to account for the duration of moist curing is given in tabular formin the ACI 209 Committee Report [1992]. This factor allows for a reduction in shrinkagewith moist curing periods greater than 7 days.Following the application of all appropriate correction factors, the shrinkage strainε sh,t (at any time t after the time t 1 in which drying begins), can be determined as afunction of the corrected ultimate shrinkage strain ε sh,u . The same hyperbolic-powerexpression used for the creep-time relationship is used, with a power of 1.0 and a timecoefficient in the denominator of 35:13

(t − t1)εsh ,t= ⋅ε sh ,u...........................Equation 2.1335 + (t − t 1)The coefficient 35 is intended for use with moist-cured concrete, and should bereplaced with 55 for steam-cured concrete. The form of Equation 2.14 was suggested byBranson et. al. [1971], and the coefficients were determined as average values from a setof 95 experimental tests. A suggested range of values for the general form of theshrinkage-time equation, given in Equation 2.14, is provided in the ACI 209 CommitteeReport:(t − t )ε sh ,t=f + (t − t 1)e1e⋅ε sh ,u.....................Equation 2.14Other design-oriented prediction models for shrinkage include the 1990 CEB model[1991] and the simplified BP (Bazant-Panula) model [1980]. The CEB model is similar tothe ACI 209 approach, and includes considerations for the effects of concrete strength,cement type, relative humidity, and member size. Concrete strength is not meant to be avariable itself, but is included to represent the effects of water-to-cement (water-tobinder)ratio and water content, since most designers will not know these mixcomposition parameters [Muller, H.S., 1992]. Unlike the ACI 209 approach, the effectsof member size on the rate of shrinkage are considered in the CEB model. The simplifiedBazant-Panula model is a bit more complex, and considers several mix compositionparameters, including sand-to-aggregate ratio, gravel-to-sand ratio, and water-to-cement(water-to-binder) ratio. The BP model also considers the interrelation of creep andshrinkage.2.3 Coefficient of Thermal ExpansionThe coefficient of thermal expansion of concrete is a function of the coefficients ofboth the aggregate and paste. However, because aggregates generally make up the bulk ofthe concrete mix, the coefficient of thermal expansion of concrete is most influenced bythe coefficient of the aggregate, as well as the quantity of aggregate in the mix. Thecoefficients of individual aggregates vary greatly with mineralogical composition, butrange from about 4 to 13 µε/°C (2.2 to 7.2 µε/°F). Values for various aggregates are14

given by Mindess and Young [1981]. The coefficient of thermal expansion for cementpaste is substantially higher than for aggregates, such that the resulting coefficients ofexpansion for concrete will be higher than for the aggregate alone.Mindess and Young **report** a range of coefficients of thermal expansion for concreteof 7.4 to 13 µε/°C (4.1 to 7.3 µε/°F). ACI Committee 209 [1992] suggests a range of 8.5to 11.7 µε/°C (4.7 to 6.5 µε/°F) be used for ordinary thermal stress calculations in theabsence of known data, with an average value of 10.0 µε/°C (5.5 µε/°F). An averagecoefficient of 11 µε/°C (6 µε/°F) is specified by AASHTO for use in all calculations[1994, 1998 and 1996].There is little data available on the coefficient of thermal expansion for highstrength or high performance concretes. It is suggested, however, that the thermalproperties of high strength concretes are similar to those of conventional concretes [ACI209, 1992].Moisture content is also known to have a significant effect on the coefficient ofthermal expansion for concrete [Mindess, 1981 and Neville, 1981]. The coefficient isminimum in the unsaturated or fully saturated conditions, and is maximum atintermediate moisture conditions. The influence of moisture content is a result of theinternal rearrangement of water molecules between capillary and gel pores as temperatureincreases. This rearrangement of water adds an additional component of expansion underincreasing temperatures, leading to a higher coefficient of thermal expansion. Since therearrangement of water molecules is not possible in the unsaturated and fully saturatedconditions, the coefficient of thermal expansion is minimized in these cases.15

3. MATERIAL FABRICATION AND DESIGN3.1 Specimen Fabrication and DesignTwelve long specimens were cast from sampled concrete on the date of the deckcasting, in four groups of samples, each sample approximately one hour after each other.For denomination of the specimens the following was used: The first number designatesthe group ID, and the second number identifies the particular specimen from that samplegroup. The specimens with identication numbers are listed in Table 3.1. All of them wereair cured. In the beginning we used the twelve specimens for shrinkage readings, as thisstarted before the CTE and creep test. One creep specimen, specimen 1-1 cracked duringshipment, but it could still be used for shrinkage measurement. Also one CTE testspecimen cracked, but since one additional specimen was fabricated for each required testin the event of shipment damage, this didn’t impact the research in any fashion. TheTable 3.1 lists each individual test and specimen identification number.Table 3.1 Specimens for C/S/TTestSpecimensCreep 2-1, 3-1, 4-1Shrinkage 1-1, 1-2, 1-3, 2-1, 2-2, 2-3, 3-1, 3-2, 3-3, 4-1, 4-2, 4-3CTE 1-3, 2-3, 4-3Creep tests were performed on eleven specimens. ASTM C512 test procedure wasfollowed with a few basic modifications, including the use of 100 x 600 mm (4 x 24 in)cylinder specimens. This specimen diameter was consistent with that used for testing ofcompressive strength and modulus of elasticity, and assured that the applied loadsrequired for testing were within the range of loads possible using equipment available tothe researchers. The length of these specimens allowed for the measurement of surfacestrains during the test using a DEMEC mechanical strain gauge with a 200 mm (8 in.)gauge length. In addition, the use of a single long specimen instead of stacking multipleshort specimens, such as three 100 x 200 mm (4 x 8 in.) cylinders, eliminated difficultieswith alignment between specimens during loading.16

In general, a total of eight or nine test specimens were cast for each mix. Two ofthese specimens were loaded for measurement of creep strains. Three specimens werekept unloaded to monitor strains due to drying shrinkage and changes in the testingenvironment, and two specimens were used for determination of the coefficient ofthermal expansion. One or two additional specimens were cast in case any of thespecimens were damaged or poorly fabricated.Specimens for each mix were cast alongside the member at the precast plant oralongside the structure at the jobsite. Precut segments of PVC pipe and speciallyfabricated aluminum end inserts were used to form the specimens. Concrete was placedin 100 to 150 mm (4 to 6 in.) layers and each layer was rodded 25 times. A set ofcreep/shrinkage/thermal (C/S/T) specimens, as well as a group of standard cylinders fortesting of compressive strength and modulus of elasticity, is shown shortly after casting atthe jobsite in Figure 3.1. For the deck, the long cylinders cast for creep (C), shrinkage (S)and coefficient of thermal expansion (T) were damaged during transportation to UMRdue to a vehicular accident. Therefore, for deck concrete, three 100 × 200 mm (4 × 8 in.)cylinders were stacked as one creep specimen. The broken long specimen could still beused for shrinkage measurement. The length of these specimens allowed for themeasurement of surface strains during the test using a DEMEC mechanical strain gaugewith a 200 mm (8 in.) gauge length.Specimens were capped to prevent moisture loss and were stored alongside thestructure for 8 to 18 hours and were shipped to the laboratory in UMR. Approximately 24hours after casting of the specimens, the PVC molds were removed and DEMECmechanical strain gauge points were fixed to the surface of the specimen using a quicksetepoxy gel. Points were placed as shown in Figure 3.1, such that three surface strainmeasurements were taken on three “sides”, 120° apart, for a total of nine strainmeasurements per specimen. The specimens were then sulfur capped to ensure smoothends, and the DEMEC points allowed setting overnight.17

4′′4′′24in 4′′4′′4′′31BACPlan View2(Diameter = 4 in)A, B and C are 120degrees apart4′′Figure 3.1 C/S/T Specimens and DEMEC Points ArrangementThe loading frames for the creep test are shown in Figure 3.2. They wereconstructed in accordance with the creep test specification of ASTM. The principle of thedesign is to apply a constant load to a stack of cylinders between two steel plates byapplying pressure with a pump beneath the lower plate and then locking in the load.Four sets of coil springs were used to each creep rig to maintain the load nearlyconstant as the specimens shortened. The springs had a maximum compression of 50 mm(2 in.) with an approximate stiffness of 1.612 kN/mm (9.205 k/in). The spring has aninside diameter of 108 mm (4.25 in.) and an outside diameter of 178 mm (7.0 in.). Thus,the total stiffness of the four set of springs was 6.448 kN/mm (36.82 k/in). The rig wasdesigned to support another set of spring so that capacity of the frame can support higherstrength concrete at a future time.18

38 .1040.2638. 1076.2050.80330254Top Plate76Ø108Ø178ThreadbarGrade 75 #87682676 7676406NutSpringBottom PlateAØ3051127 12740676Middle Plate1867SECTION A-A20376406CouplerChannelC 5x6.7Jack Plate267381622330LOADING FRAME25440676Middle and Bottom Plates(Uni ts: mm)Figure 3.2 Creep Loading Frame and SpecimensA jack and a load cell were used to stress the creep rigs (as shown in Figure 3.3).When the correct load was reached, the nuts below the bottom plate were tightened. Thespecimens for the HPC girder mix were loaded 2 days after casting to 40% of nominaldesign compressive strength of the mix. For the cast-in-place specimens, one was aircured in the testing room and the other was moist cured prior to be loaded at 28 days.19

Figure 3.3 Creep Loading Frame and SpecimensThe applied load for each specimen was maintained throughout the tests using testframes. The loss of load with time, due to the shortening of the specimens andconsequential elongation of the springs could be determined by monitoring the springelongation since the stiffness of the springs was know. When 2% of the initial load waslost, the load was reapplied using the pump and ram.Readings were taken every day for the first week after loading, every few days forthe first 28 days and every few weeks thereafter.Strains were monitored on the two loaded specimens and three unloaded specimensfor each mix. The creep strain for each loaded specimen was determined by subtractingthe average strain on the unloaded specimens from the measured strain on the loadedspecimen. Measurements were taken every few days for approximately the first 28 days,and every few weeks thereafter for a total duration of at least 180 days.Shrinkage tests were performed on the sampled mix. Tests were performed inparallel with the creep tests for the mix, and essentially involved the measurement oftime-dependent strain on unloaded specimens. Three specimens were typically used foreach mix.As discussed, specimens were transported from the precast plant or jobsite at earlyages. Cylinder molds were removed approximately 24 hours after the specimens werecast, and the first strain measurements were typically taken about 24 hours later. The 2420

Table 3.2 Mix Constituents and Proportions for Bridge A6130 and A6671Mix Proportions Deck mix A 6130[Myers and Yang,2004]CoarseAggregateTypeGrad D porphyryfor PCCP & MasonryDeck mix A 6671[MoDOT Report RI01-044,2003]Potosi Dolomite from SullivanQuantity lbs/cy 1684 1868Fine Aggregate Type Class A Natural Sand Little Piney RiverQuantity lbs/cy 1078 1080Water Type Potable PotableQuantity lbs/cy 290 258.7Cement Type Type I Buzzi Unicem (Type I)Quantity lbs/cy 558 390Fly Ash Type Class C Labadie, Mineral resource Tech.Quantity lbs/cy 105 98Microsilica Type MicrosilicaQuantity lbs/cy 42 N.A.Retarder Type 300 RQuantity lbs/cy 20 N.A.Air Entrainment Type Not **report**ed Not **report**edQuantity lbs/cy 6 6HRWR Type Not **report**edQuantity oz/cy 25 N.A.GGFBS Type --Buzzi UnicemQuantity lbs/cy N.A. 163w/cm ratio 0.41 0.39N.A. – Not Applicablew/cm – water to cementitious ratio------24

4. EXPERIMENTAL RESULTS4.1 Results for Creep Test (Bridge Deck A6671)This section focuses on the individual and combined behavior of the testedspecimens for creep for bridge deck mix A6671. For the concrete deck, strain wasmeasured before and after loading to determine the elastic strain during loading. The rawdata obtained from creep tests (for bridge deck mix A6671) was plotted to understand thebehavior of each individual specimen and then averaged for three specimens (see Section3.1). The raw data obtained from creep tests (for bridge deck mix A6671) was then curvefitted for comparison purpose with that of the bridge deck mix of A6130. The primarypurpose of this comparison study was to understand the creep and shrinkage behavior ofthe two bridge deck mixes.Figure 4.1 below shows the individual behavior of the three specimens (asdiscussed in experimental test section, chapter 3) instrumented and evaluated for creep.The raw data (of bridge deck mix A6671) obtained from the experiments creep frames isused for plotting and no curve fit is applied to this figure. It is evident from Figure 4.1that there is irregularity in the graphs over time. This is due to temperature fluctuation inthe structural engineering laboratory where the specimens were monitored during themonitoring period.700600creep coeffic i ent500400300200100Specimen 2Specimen 3Specimen 406/28/03 10/6/03 1/14/04 4/23/04datesFigure 4.1 Individual Behaviors of Three Creep Specimens (Raw Data)25

Figure 4.2 illustrates the combined behavior of the three specimens evaluated forcreep (of bridge deck mix A6671) with raw data and the curve fit. For plotting Figure 4.2the average value of the raw data for the three specimens was taken and the curve fittingwas done using Equation 4.1.creep coeff.21.81.61.41.210.80.60.40.200 100 200 300daysCombined CreepCurve (Raw Data)Combined CreepCurve (Curve Fit)Figure 4.2 Combined Behaviors of Three Creep Specimens (Raw and Curve fit Data)There are three forms of Equations investigated for curve fitting, namely a generalfit, power fixed and parameter fixed. Details on each of these curve fitting methodologiescan be referenced in the previous study by Myers and Yang [2004]. Among these thegeneral form was selected because of its improved curve fitting characteristics. Equation4.1 is the general form equation used for curve fitting and Table 4.1 shows the resultingbest fit curve data parameters used in the equation. The value of R 2 obtained from thefitted curve was 0.956.C ct=c(t-t0)d + (t-t ) 0cC .....................Equation 4.1cuwhere, C ct is the creep coefficient at time t, C cu is the ultimate creep coefficient, c and dare constants.26

Table 4.1 Creep-Time Regression Curve Parameters (General Form)General Form of Equation 4.1Bridge deck mix c d C cu R 2A 6671 0.6 10 2.4 0.95584.2 Results for Shrinkage Test (Bridge Deck A6671)In this section the results for individual and combined behavior of four shrinkagespecimens of bridge deck mix A6671 are plotted (see Section 3.1). The readings weretaken for the four specimens at regular intervals. The raw data obtained from shrinkagetest (for bridge deck mix A6671) was plotted to understand the behavior of the specimensindividually and also in combination. For the comparison and better understandingpurpose the raw data is curve fitted.Figure 4.3 shows the individual behavior for the four individual specimens ofbridge deck mix A6671 (see Chapter 2) evaluated for shrinkage; the raw data was used inplotting the figure and no curve fit is applied.shri nkage stra i700n60050040030020010000.00 20.00 40.00 60.00 80.00 100.00daysSpecimen 1Specimen 2Specimen 3Specimen 4Figure 4.3 Individual Behaviors of 4 Shrinkage Specimens for Deck A6671(Raw Data)27

Figure 4.4 shows the combined behavior of shrinkage specimens (of bridge deckmix A6671) with the raw data and the curve fit. Curve fit was done using Equation 4.2and the parameters are listed in Table 4.2As mentioned in the Section 4.1, among the three types of regression analysis,general form was used as it fits the data best. Equation 4.2 was used to curve fit the rawdata. Table 4.2 shows the parameters used for general fit and the value of R 2 wasobtained from the fitted curve.ε =sh ,te(t-t1)ε e shu..................Equation 4.2f (t-t )+1where, ε sh,t is the shrinkage at time t, ε sh,u is the ultimate shrinkage of concrete, e and f areconstants.Table 4.2 Shrinkage-Time Regression Curve Parameters (General Form)General Form of Equation 4.2Average for e f ε sh,u R 2HPC Girders 1 21 410 0.9765shrinkage strain450.00400.00350.00300.00250.00200.00150.00100.0050.000.000.00 100.00 200.00 300.00 400.00daysShrinkage Curve(Raw Data)Shrinkage Curve(Curve Fit)Figure 4.4 Combined Behaviors of Four Shrinkage Specimens (Raw Data and Curve Fit)28

4.3 Test Results for CTE TestThe Coefficient of Thermal Expansion (CTE) of concrete is a function of thecoefficients of both the aggregate and the paste. However, aggregates generally make upthe bulk of the concrete mix constituents and therefore the coefficient of thermalexpansion of concrete is most influenced by the coefficient of the aggregate, as well asthe quantity of aggregate in the mix.There were 3 specimens (bridge deck mix A 6671) evaluated for coefficient ofthermal expansion (see Section 3.1) and the average value of coefficient of thermalexpansion was calculated as follows:: α t = 5.27 x 10 -6 1/F (9.48x10 -6 1/C). Furtherdiscussion about the CTE is presented in Chapter 5.29

5. COMPARISION OF BRIDGE DECK MIX A6671 TO A61305.1 Comparison for Creep ResultsThis chapter discusses the comparison of the results for creep, shrinkage andcoefficient of thermal expansion for the sample specimens taken from the bridge deckmixes for Bridges A6671 and A6130.Table 5.1 shows the creep comparison of the various parameters used in curvefitting and the corresponding R 2 values obtained from the best fit curve for the two bridgedeck mixes A6671 and A6130 investigated (see Table 4.1 and 4.2). The values for bridgedeck mix A6130 were previously **report**ed by Myers and Yang (2004) and the values forbridge deck mix A6671 were obtained by curve fitting the raw data obtained fromexperiments (see Section 4.1 and 4.2) conducted in this study. Parameters, for curvefitting of both bridge deck mixes were obtained using Equation 4.1 and 4.2 (generalform). The value of R 2 for bridge deck mix A6671 is lower than that of the bridge deckmix A6130. The difference in correlation values may be primarily attributed to thegreater degree of temperature variation during monitoring in the laboratory and the widerange of raw data obtained in the experiment of bridge deck mix A6671. However, itshould be noted that both R 2 values are quite high indicative of a high level of curve fit.Table 5.1 Comparison of Creep-Time Regression Curve Parameters (General Form)Bridge deckmixc d C cu R 2A6671 0.6 10 2.4 0.954A6130 0.4 8.4 4.53 0.993Figure 5.1 shows comparison of creep coefficients obtained for the HPC deck mixfrom Bridge A6671 to that of Bridge A6130. The relationship which is shown for bothbridge deck mixes represents a comparison of the curve fit equations obtained based onexperimental data.30

2.52creep coeff.1.51BRIDGE A 6130 HPC0.50-0.5 0 100 200 300 Deck Mix (Curve Fit)BRIDGE A 6671 HPCDeck Mix (Curve Fit)daysFigure 5.1 Creep Comparison CurveFrom the curve fit equations shown in Figure 5.1, the creep coefficient value forbridge deck mix A6671 is 1.78 and for bridge deck mix A6130 is 2.21. The creepcoefficient for bridge deck mix A6671 was 19.3% lower than that of the bridge deck mixA6130. As discussed earlier (see Section 1.1) the factors affecting the creep coefficientare largely dependent on mix composition, curing conditions, loading conditions, watercement ratio and others. As observed from the mix constituents and proportions (seeSection 3.2), the coarse aggregate was 9.9% higher in bridge deck mix A6671 comparedto that of bridge deck mix A6130. Since creep occurs in the paste of concrete and theaggregate tends to restrain it, a lower creep value for bridge deck mix A6671 wassomewhat expected and was the case. Moreover, creep is largely influenced by thecement content and w/cm ratio, therefore in general the higher the cement content andw/cm ratio, the higher the creep coefficient. The cement content and the w/cm ratio werehigher in bridge deck mix A6130 than that for bridge A6671, resulting in higher value ofcreep coefficient.5.2 Comparison of Shrinkage ResultsTable 5.2 shows the comparison of the shrinkage parameters used in the curve fitequation (see Section 4.2) and the R 2 values obtained from curve fitting for the twobridge deck mixes. The values for bridge deck mix A6130 were previously **report**ed by31

Myers and Yang (2004) and the values for bridge deck mix A6671 were obtained bycurve fitting the raw data obtained from experiments conducted in this study. The valueof R 2 for bridge deck mix A6671 is comparable to that of the bridge deck mix A 6130.Table 5.2 Comparison of Shrinkage-Time Regression Curve Parameters (General Form)Bridge mix e f e shu R 2A 6671 1.0 21 410 0.977A 6130 1.0 20.8 454 0.987Figure 5.2 compares the shrinkage results for the HPC deck mix Bridge A6671 tothat of Bridge deck mix A6130. The relationship which is shown for both bridge deckmixes represents a comparison of the curve fit equations obtained based on experimentaldata. It can be observed from Figure 5.2 that the shrinkage strain values for bridge deckmix A6671 was 367.16 and for the bridge deck mix A6130 was 406.97. Shrinkage strainof bridge deck mix A6671 was 9.8% lower than the bridge deck mix A6130. Asdiscussed earlier (see Section 1.1), factors affecting shrinkage include mix composition,curing conditions, member size and shape, water cement ratio etc. As observed from themix constituents and proportions (see Section 3.2), the coarse aggregate content was9.9% higher for deck mix A6671 compared to that of deck mix A6130. The courseaggregate tends to restrain the paste matrix such that a lower shrinkage strain for deckmix A6671 was somewhat expected and consistent with the test results. Moreover, thew/cm ratio was also an influencing factor for shrinkage, with lower ratios resulting inconcrete with lower shrinkage. The w/cm ratio was also lower for deck mix A6671compared to that of deck mix A6130, resulting in a lower value of shrinkage strain.32

shrinkage strain4504003503002502001501005000.00 100.00 200.00 300.00 400.00daysBRIDGE A 6130HPC Deck Mix( Curve Fit)BRIDGE A 6671HPC Deck Mix( Curve Fit)Figure 5.2 Shrinkage Comparison Curve5.3 Comparison of CTE ResultsTable 5.3 and Figure 5.3 illustrate a comparison of CTE results for HPC deck mixA6671 to that of deck mix A6130. In both cases the values are based on laboratorytesting of concrete sampled during placement of concrete. The result shows that the valueof CTE for bridge A6671 was 3.46% lower than deck mix A6130. The value of CTE fordeck mix A6130 was previously **report**ed by Myers and Yang [2004]. The CTE value fordeck mix A6671 was obtained from laboratory tests. The variation in CTE seems to bedue to the higher amount of coarse aggregate and slag in the deck mix of A6671. TheCTE is a function of both the aggregate and the paste. Aggregates generally makes upbulk of the concrete mix and have a higher modulus therefore generally influencing theCTE more significantly. The CTE value is also affected by moisture content. Themoisture (water) content is higher in bridge deck mix A6130 also possibly contributing tothe slightly higher value of CTE. As the test results for Bridge A6130 is slightly higher,stresses due to thermal expansion and contraction could be expected to be slightly higher.Table 5.3 Average value of CTE for both bridge mixesAveragevalue ofCTECTE for A 6130 CTE for A 66711/°F 1/°C 1/°F 1/°C5.46x10 -6 9.83 x10 -6 5.27 x10 -6 9.48 x10 -6 33

5.55.455.45.355.35.255.2BRIDGE A 6671HPC Mix Design ( RawData)BRIDGE A 6130HPC Deck Mix( Curve Fit)5.15µe/°FFigure 5.3 CTE Comparison Curve34

6. CONCLUSIONS AND RECOMMENDATIONSThis chapter outlines the conclusions based on the testing of specimens for bridgedeck mix A6671 and the comparative study of this with bridge deck mix A6130.The following conclusions were based on the observations from creep, shrinkageand CTE test results of specimens from deck mix A6671:1. The creep coefficient for deck mix A6671 at 180 days (after curve fitting) was1.78.2. The shrinkage strain (µε) at 180 days (after curve fitting) was 367.2.3. The coefficient of thermal expansion, α t was observed to be 5.27 x 10 -6 1/F(9.48x10 -6 1/C).The following conclusions were based on the comparison study between deckmixes A6130 and A6671:1. The creep coefficient for deck mix A6671 was 19.3% lower than that of thebridge deck mix A6130. The reason for this higher difference in the creepcoefficient may be associated with the higher (9.9%) amount of coarse aggregate,lower amount of cement content and lower w/cm ratio in deck mix of A6671. Asnoted previously, creep is affected by the aggregate in the concrete, paste matrix,and the w/cm ratio among other factors. Therefore, a higher coarse aggregatecontent and lower w/cm ratio can be expected to result in a lower creepcoefficient, as was the case.2. Shrinkage strain for deck mix A6671 was 9.8% lower than that of the bridge deckmix A6130. The reason for this was the lower w/cm ratio, lower cement contentand higher coarse aggregate content in deck mix A6671. Based on studies we cansay that in general lower w/cm ratio with reduced cement content and more coarseaggregate will result in less creep and less shrinkage.3. CTE for bridge deck mix A6671 is 3.5% lower than that of the bridge deck mixA6130. This apparent variation may be attributed to the difference in the quantityof the coarse aggregates and moisture content used in both mixes.4. The new deck mix developed by MoDOT and used in Bridge A6671 appears tohave preferable SH, CR, and CTE characteristics for a bridge deck application35

when compared to the mix design used for Bridge A6130. A reduction in cementfor bridge deck applications can aid in reducing or eliminating shrinkage relatedcracking problems and high stresses developed due to thermal expansion andcontraction.The following recommendations were based on the comparison study between deckmixes A6130 and A6671:1. A reduction in the cement content for bridge deck applications is recommendedbased on the mix designs investigated in this study to aid in reducing oreliminating shrinkage related cracking problems.2. A higher percentage of coarse aggregate is recommended assuming placementand workability requirements can be met to aid in reducing the overall shrinkageof a concrete mix based on the mix designs investigated in this study.36

REFERENCESAmerican Association of State Highway and Transportation Officials, AASHTO LRFDBridge Design Specifications, First Edition, 1994.American Association of State Highway and Transportation Officials, StandardSpecifications for Highway Bridges, Sixteenth Edition, 1996.ACI Committee 209, “Prediction of Creep, Shrinkage, and Temperature Effects inConcrete Structures,” ACI 209R-92, American Concrete Institute, Detroit, 1992.ACI Committee 363, “State-of-the-Art Report on High-Strength Concrete,” ACI 363R-92,American Concrete Institute, Detroit, 1992.American Society for Testing and Materials, “Standard Test Method for Creep ofConcrete in Compression,” ASTM C512-87(1992)e1, ASTM, West Conshohocken,Pennsylvania, 1992.ASTM Standards C 109, “Standard Test Methods for Compressive Strength of HydraulicCement Mortars”, 2002.Bazant, Z. P. and Panula, L., “Creep and Shrinkage Characterization for AnalyzingPrestressed Concrete Structures,” PCI Journal, May/June 1980, Vol. 15, No. 3, pp.87-122.Branson, D. E. and Christiason, M. L., “Time-Dependent Concrete Properties Related toDesign – Strength and Elastic Properties, Creep, and Shrinkage,” ACI SpecialPublication SP-27, Creep, Shrinkage, and Temperature Effects in Concrete Structures,American Concrete Institute, Detroit, 1971.Branson, D. E. and Kripanarayanan, K. M., “Loss of Prestress, Camber, and Deflection ofNon-composite and Composite Prestressed Concrete Structures,” PCI Journal,September/October 1971, Vol. 16, No. 5, pp. 22-52.Brooks, J. J. and Neville, A., “Creep and Shrinkage of Concrete as Affected byAdmixtures and Cement Replacement Materials,” Creep and Shrinkage of Concrete:Effect of Materials and Environment, ACI SP 135, American Concrete Institute,Detroit, 1992, pp. 19-36.Comite Euro-International du Beton (CEB), CEB-FIP International Recommendationsfor the Design and Construction of Concrete Structures, Paris-London, 1970.Comite Euro-International du Beton (CEB), CEB-FIP Model Code 1990, Final Draft,Lausanne, 1991.37

CTE Quarterly Report, “Creep, Shrinkage and CTE Evaluation”, September 2003, RI00002B.Myers, J.J., and Yang, Y., “Field and laboratory Performance of Prestressed ConcreteGirders for MO Bridge Structures”, MODoT, RDT -04-016, June 2004.El Hindy, E., Miao, B., Chaallal, O., and Aitcin, P.-C., “Drying Shrinkage of Ready-Mixed High Performance Concrete,” ACI Materials Journal, May/June 1994, Vol. 91,No. 3, pp. 300-305.Gilbert, R. I., Time Effects in Concrete Structures, Elsevier Science Publishers,Amsterdam, 1988.Hansen, T. C. and Mattock, A. H., “Influence of Size and Shape of Member on theShrinkage and Creep of Concrete,” ACI Journal, February 1966, Vol. 63, No. 2, pp.267-289.Hanson, J. A., “Prestress Loss as Affected by Type of Curing,” PCI Journal, April 1964,Vol. 9, No. 2, pp. 69-93.Klieger, P., Some Aspects of Durability and Volume Change of Concrete for Prestressing,Research Development Bulletin 118, Portland Cement Association, Skokie, Illinois,1960.Libby, J. R., Modern Prestressed Concrete, Fourth Edition, Van Nostrand Reinhold, NewYork, 1990.McDonald, D., “Development of a Simplified Code Procedure for the Prediction ofShrinkage and Creep,” Creep and Shrinkage of Concrete – Proceedings of the FifthInternational RILEM Symposium, International Union of Testing and ResearchLaboratories for Materials and Structures (RILEM), Cambridge, 1993.Mindess, S. and Young, J. F., Concrete, Prentice-Hall, Englewood Cliffs, New Jersey,1981.MoDOT, “Laboratory Study – Laboratory Testing of Bridge deck Mixes”, RI01-044,March 2003Muller, H. S., “New Prediction Models for Creep and Shrinkage of Concrete,” Creep andShrinkage of Concrete: Effect of Materials and Environment, ACI SP 135, AmericanConcrete Institute, Detroit, 1992, pp. 1-18.38

Nasser, K. W. and Al-Manaseer, A. A., “Creep of Concrete Containing Fly Ash andSuperplasticizer at Different Stress/Strength Ratios,” ACI Journal, July/August 1986,Vol. 83, No. 4, pp. 668-673.Neville, A. M., Dilger, W. H., and Brooks, J. J., Creep of Plain and Structural Concrete,Longman Group, 1983.Neville, A. M., Properties of Concrete, Third Edition, Pitman Publishing, London, 1981Ngab, A. S., Nilson, A. H., and Slate, F. O., “Shrinkage and Creep of High StrengthConcrete,” ACI Journal, July/August 1981, Vol. 78, No. 4, pp. 255-261.Nilson, A. H. and Winter, G., Design of Concrete Structures, Eleventh Edition, McGraw-Hill, New York, 1991.Parrot, L. J., “The Properties of High-Strength Concrete,” Technical Report No. 42.417,Cement and Concrete Association, Wexham Springs, 1969.Sennour, M. L. and Carrasquillo, R. L., Creep and Shrinkage Properties in ConcreteContaining Fly Ash, Research Report 481-6, Center for Transportation Research, TheUniversity of Texas at Austin, Austin, Texas, 1989.Smadi, M. M., Slate, F. O., and Nilson, A. H., “Shrinkage and Creep of High-, Medium-,and Low-Strength Concretes, Including Overloads, ACI Materials Journal, May/June1987, Vol. 84, No. 3, pp. 224-234.Swamy, R. N. and Anand, K. L., “Shrinkage and Creep Properties of High StrengthStructural Concrete,” Civil Engineering and Public Works Review (London), October1973, Vol. 68, No. 807, pp. 859-868.Chojnacki, T., MoDOT Mix Design **report**, Tuesday June 22, 2004 via emailcorrespondence.Troxell, G. E., Davis, H. E., and Kelly, J. W., Composition and Properties of Concrete,Second Edition, McGraw-Hill, New York, 1968.39